Embed Size (px)
THE ROLE OF NIOBIUM IN AUSTENITIC AND DUPLEX STAINLESS STEELSDavid Dulieu Consultant, 20 Topside, Grenoside Sheffield, S35 8RD, United Kingdom
Abstract The two principal roles of niobium in cast and wrought austenitic stainless steels are as a stabilising agent to reduce the risk of intergranular corrosion and as a strengthening agent. To date there appears to be no parallel roles in the duplex, austenitic-ferritic stainless steels. The principles for designing an austenitic steel composition are outlined and the effects of niobium as an alloying element summarised. The characteristics of the principal precipitate phases and their occurrence are reviewed in the context of service requirements, to illustrate how compositions have evolved. Metallurgical developments covered include the benefits derived from a balanced reduction in the levels of niobium and carbon in the 347 composition. Application of controlled heat treatments combined with cold working has allowed optimisation of both steam-side oxidation and creep strength for this widely used grade. The combination of low levels of niobium with enhanced nitrogen additions has led to alternative stabilisation mechanisms. Enhanced precipitation strengthening for high temperature applications derives from multiple microalloying additions of, principally, niobium, titanium and vanadium and recognition of the role of the chromium-niobium nitride. Families of high strength creep resisting steels have been developed for both fossil and nuclear power generation applications, based on the synergistic effects of multiple alloying additions of molybdenum, niobium, titanium, nitrogen, copper and tungsten. These steels exploit knowledge of alloy design to combine effective solid solution and precipitation strengthening with optimum grain boundary precipitation.
Introduction Background and History The majority of niobium-bearing austenitic steels fall into two major classes: steels with stabilising additions to prevent intergranular corrosion and compositions for elevated temperature service. The latter can be subdivided into those with niobium as the principal addition enhancing creep strength, and more complex alloys using the interactive effects of other additions. Although this review covers primarily wrought alloys, many individual grades are available as castings. The development of the niobium-bearing steels has been linked closely to applications within power generation, chemicals, nuclear and gas turbine technologies. Binder (1) gave a comprehensive review of the field in 1957, a time when adoption of the 347 grade in the superheater and other high temperature areas of steam power plant had focused attention on several issues. These included hot-workability, problems of liquation and stress-relief cracking on welding and cast and product form variability of elevated temperature properties. By the time of the review by Keown and Pickering (2) in 1981, the variability in behaviour of niobium-bearing steels was in large measure understood. The importance of the temperature and compositional dependence of the solubility of Nb(C,N) was established and effects of supersaturation, cold work, and ageing or stabilising heat treatments on secondary precipitation had been related to the behaviour of weld and parent metals. The present review does not attempt to cover all the more recent compositional variants or applications. The starting-point is to consider the selection of the basic iron-chromium-nickel(manganese-nitrogen) matrix, within which niobium will play its role. Examples of the various niobiumcontaining compositions are then introduced. The effects of niobium as an alloying element are summarised and the precipitate phases and precipitation sequences in both wrought and cast alloys outlined in relation to service requirements. Aspects of oxidation and the role of niobium in steels subject to irradiation are then considered. Unless specified, descriptions of steels such as 347 used in this text are generic terms and not specific, standardised grade descriptions; the references cited should be consulted for further details. All compositions are given in weight %. Metallurgical Developments Important metallurgical aspects of developments in niobium-bearing steels which are reflected in the work reviewed fall under the following headings : The benefits for hot workability, ductility and weldability to be gained from minimising the volume fraction of primary carbide particles. The importance of additional carbide-forming elements such as titanium in extending the effectiveness of the niobium-based MC precipitates in high temperature steels. Recognition of the significant effects of low levels of niobium additions, especially when present in steels with enhanced nitrogen levels, in relation to strength and intergranular corrosion resistance. The exploitation of mixed intragranular precipitate populations for creep strength. The stability of Nb(C,N) versus the Z-phase (Cr,Nb) nitride and secondary chromium carbides in relation to strengthening effects in the higher nitrogen steels. Control over precipitate distribution and the balance between inter- and intragranular precipitation. This to optimise creep rupture life, in both low and high carbon-niobium alloys across a range of service temperatures. Optimisation of the roles of alloying elements in irradiated microstructures.
The Iron-Chromium-Nickel Matrix and the Roles of Alloying Elements Found in Austenitic and Duplex Stainless Steels Austenitic Steels The basic physical metallurgy of austenitic stainless steels has been summarised by Harries (3). Stainless steels have chromium as their principal addition. In austenitic stainless steels the effective lower limit is around 13%. The upper limit rarely exceeds 25% and is set by the tendency to form the sigma Fe-Cr intermetallic phase on thermal exposure, or the behaviour of high chromium steels in specific aggressive environments. Silicon and aluminium promote oxidation resistance and are ferrite stabilisers. Rare earth additions may be used to improve oxide stability. For elevated temperature strength additions of nitrogen, molybdenum and tungsten are used, together with elements forming stable intragranular precipitates on a scale inhibiting dislocation movement. For corrosion resistance at relatively low temperatures, the protective, passive oxide film must not be weakened by localised matrix chromium depletion. A decision will be made, based on fabrication route and service exposure, on the need for a stabilising addition of either titanium or niobium versus use of a low carbon grade. Pitting resistance is enhanced by additions of molybdenum, tungsten and nitrogen. Having established an oxidation or corrosion-resistant composition, a nickel addition, or less often a combined nickel-manganese-nitrogen addition, can then be chosen to promote the formation of an austenitic structure. Factors determining the level of austenite stabilisers include: Hot workability considerations, the need for a controlled solidification path. Stability of the structure in respect of transformation during work-hardening and at low temperatures, need to achieve low magnetic permeability. The beneficial effects of nickel for reducing carburisation and nitridation rates. Susceptibility to sigma phase formation and changes in matrix and grain boundary region compositions arising from precipitation at elevated temperatures.
The matrix compositions of most of the niobium-bearing steels fall in the ranges 15-25%Cr, 9-35%Ni. Nickel and chromium equivalents can be used to predict solidification structures. For example, Kotecki and Siewert (4) summarised weld structure prediction models derived from the original Schaeffler Diagram and gave a factor of 0.7 for the chromium equivalent of niobium. Phase diagrams are supplemented by calculations from thermodynamic data for prediction of equilibrium phase stability. Of the minor elements in austenitic stainless steels, sulphur may segregate to grain boundaries at high temperatures and is deleterious to pitting corrosion resistance. It is kept to low levels (